DOI: 10.17188/1286171
title: Materials Data on Ca9LaMn10O30 by Materials Project

description: Ca9LaMn10O30 is Orthorhombic Perovskite-derived structured and crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are eighteen inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.74 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.72 Å. In the third Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.73 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.74 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.73 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.74 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.73 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.72 Å. In the ninth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.74 Å. In the tenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.74 Å. In the eleventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.73 Å. In the twelfth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.74 Å. In the thirteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.72 Å. In the fourteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.73 Å. In the fifteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.35–2.72 Å. In the sixteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.72 Å. In the seventeenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.74 Å. In the eighteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.32–2.72 Å. There are two inequivalent La3+ sites. In the first La3+ site, La3+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of La–O bond distances ranging from 2.36–2.90 Å. In the second La3+ site, La3+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of La–O bond distances ranging from 2.36–2.90 Å. There are twenty inequivalent Mn+3.90+ sites. In the first Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.97 Å. In the second Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 22–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.97 Å. In the third Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 22–27°. There are a spread of Mn–O bond distances ranging from 1.94–1.97 Å. In the fourth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–26°. There are a spread of Mn–O bond distances ranging from 1.92–1.97 Å. In the fifth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 24–27°. There are a spread of Mn–O bond distances ranging from 1.94–1.96 Å. In the sixth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–27°. There are a spread of Mn–O bond distances ranging from 1.92–1.97 Å. In the seventh Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 22–28°. There are a spread of Mn–O bond distances ranging from 1.93–1.96 Å. In the eighth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 24–27°. There are a spread of Mn–O bond distances ranging from 1.94–1.96 Å. In the ninth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.97 Å. In the tenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 23–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.97 Å. In the eleventh Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 24–27°. There are a spread of Mn–O bond distances ranging from 1.94–1.96 Å. In the twelfth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–28°. There are a spread of Mn–O bond distances ranging from 1.92–1.98 Å. In the thirteenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 23–28°. There are a spread of Mn–O bond distances ranging from 1.93–1.97 Å. In the fourteenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 24–28°. There are a spread of Mn–O bond distances ranging from 1.94–1.96 Å. In the fifteenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 24–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.98 Å. In the sixteenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 22–27°. There are a spread of Mn–O bond distances ranging from 1.92–1.97 Å. In the seventeenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–27°. There are a spread of Mn–O bond distances ranging from 1.92–1.97 Å. In the eighteenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–27°. There are a spread of Mn–O bond distances ranging from 1.91–1.97 Å. In the nineteenth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 23–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.98 Å. In the twentieth Mn+3.90+ site, Mn+3.90+ is bonded to six O2- atoms to form corner-sharing MnO6 octahedra. The corner-sharing octahedra tilt angles range from 20–27°. There are a spread of Mn–O bond distances ranging from 1.93–1.97 Å. There are sixty inequivalent O2- sites. In the first O2- site, O2- is bonded in a 5-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the second O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the third O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the fourth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the fifth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the sixth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the seventh O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the eighth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the ninth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the tenth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the eleventh O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the twelfth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the thirteenth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the fourteenth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the fifteenth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the sixteenth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the seventeenth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the eighteenth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the nineteenth O2- site, O2- is bonded in a 4-coordinate geometry to one Ca2+, one La3+, and two Mn+3.90+ atoms. In the twentieth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the twenty-first O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the twenty-second O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the twenty-third O2- site, O2- is bonded in a 5-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the twenty-fourth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the twenty-fifth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the twenty-sixth O2- site, O2- is bonded in a 5-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the twenty-seventh O2- site, O2- is bonded in a 5-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the twenty-eighth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the twenty-ninth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the thirtieth O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the thirty-first O2- site, O2- is bonded in a 4-coordinate geometry to two Ca2+ and two Mn+3.90+ atoms. In the thirty-second O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the thirty-third O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the thirty-fourth O2- site, O2- is bonded in a 5-coordinate geometry to two Ca2+, one La3+, and two Mn+3.90+ atoms. In the thirty-fifth O2- site, O2- is bonded in a 5-coordinate geometry to three Ca2+ and two Mn+3.90+ atoms. In the thirty-sixth O2- site, O2- is bonded in a 4-coordinate geometry to one Ca2+, one La3+, and two Mn+3.90+ atoms.